Cyclohexane oxidation using transition metal-containing aluminophosphates (MAPO-VFI)
Post on 05-Jul-2016
Embed Size (px)
JOURNAL OF MOLECULAR CATALYSIS A:CHEMICAL
Journal of Molecular Catalysis A: Chemical I 17 ( 1997) 405-4 I I
Cyclohexane oxidation using transition metal-containing aluminophosphates ( MAPO-VFI)
Fernando J. Luna, Silvio E. Ukawa, Martin Wallau, Ulf Schuchardt *
Received 19 April 1996: accepted 29 May 1996
The preparation of Co-, Cr-, Fe-, Mn-, Ti-, and V-containing aluminophosphates (MAP01 with VFI structure is described. Physico-chemical techniques were used to characterize the solids synthesized. The MAPO-VFI were compared to AIPO-VFI impregnated with the various metals confirming the isomorphous substitution of Co, Cr, Fe, and Ti into the structure. V is coordinated to defect sites and Mn probably precipitated as oxide on the crystal surface. V- and CrAPO-VFI are active catalysts for the oxidation of cyclohexane with tear-butyl hydroperoxide producing cyclohexanone with some cyclohexanol and cyclohexene. CrAPO-VFI was recycled twice without significant loss of activity. On the other hand. VAPO-VFI showed significant metal leaching.
Keywords: VPI-5: Metallaluminophosphates; VFI-structure; Cyclohexane: Catalytic oxidation; terr-hutyl hydroperoxide
Right after his account of the first synthesis of an aluminophosphate molecular sieve with channels formed by 18 atom rings and pore diameters of 1.2 nm [ 11, Davis et al.  found that it was possible to isomorphously substitute silicon and cobalt into its framework. The new molecular sieve was named VPI-5, and the IZA eventually decided upon the symbol VFI to describe its structure. In this work, the alu- minophosphate VPI-5 will be referred to as AlPO-VFI. VPI-5 containing other isomor- phously substituted metals M will be called
Corresponding author. Fax: + 55-19-2393805; e-mail: firstname.lastname@example.org.
MAPO-VFI. Since Davis discovery, the incor- poration of small amounts (less than 5% wt/wt> of metals such as magnesium , iron [4,5], and cobalt , which substitute aluminum isomor- phously, has been reported. The incorporation of manganese into AlPO-VFI has been pub- lished as well , but isomorphous substitution is unlikely. Although much energy has been devoted to the study of synthesis conditions and the characterization of AlPO-VFI, only a few reports [6,7] can be found on its use, or on the use of MAPO-VFI, in catalysis, probably be- cause of its relative thermal instability. For molecular sieves with the VFI structure. the removal of zeolitic water is an essential step that has to be done prior to any application-ori- ented studies such as catalysis. The thermal
1381 -I 169/97/$17.00 Copyright 0 1997 Elsevier Science B.V. All rights reserved /If S138l-1169(96)00271-3
406 F.J. Luna et al. /Journal of Molecular Catalysis A: Chemical 117 (1997) 405-41 I
treatment requires carefully controlled condi- tions, otherwise the VFI structure will readily decay to the AlPO-8 phase [8,9].
Transition metal-containing aluminophos- phates have great potential as heterogeneous oxidation catalysts for a variety of organic sub- strates [lo]. MAPO-5 (AFI structure), a more stable aluminophosphate with a smaller pore diameter (0.73 nm), has been successfully ap- plied in the oxidation of alkanes, as reported for CoAPO-5 [II], VAPO-5 [12,13], CrAPO-5 , and TiAPO-5 . The use of MAPO-VFI takes advantage of the known catalytic properties of metallaluminophosphates combined with a larger pore diameter, allowing the processing of bulkier organic molecules.
This work describes the synthesis of the novel aluminophosphates TiAPO-VFI, VAPO-VFI, and CrAPO-VFI, an$ reports their catalytic ac- tivity in the oxidation of cyclohexane in com- parison with Mn-, Fe-, and Co-containing AlPO-WI, and with AlPO-VFI impregnated with Cr and V.
2.1. Synthesis of the catalysts
MAPO-VFI were synthesized according to a modified version of the published procedure : Pseudoboehmite (Condea), phosphoric acid (Al- drich) and distilled water were mixed in a molar ratio of 1: 1:40 and aged for 2 h. One equivalent of di-n-propylamine (Aldrich) was added and the gel aged for another 2 h. The metal source, 0.04 equivalents of Mn(CH,COO), . 4H,O (Fluka), Co(CH ,COO), . 4H 2O (Fluka), VOSO, 3 3H,O (Aldrich), Cr(NO,), .9 H,O (Aldrich), or FeCl,, (Aldrich), was dissolved in ca. 5 ml of water and added to the gel, which was vigorously stirred for 15 min. For the syn- thesis of TiAPO-WI, Ti(C,H,O>, (Aldrich) dissolved in ethanol (Ti - 20%) was added to the gel. The gel was then transferred to a teflon-lined autoclave and crystallized by heat-
ing at 150C for 3.5 h. The crystals were sepa- rated from the remaining gel by washing with plenty of distilled water on a 250 Tyler mesh sieve. After filtration, the crystals were dried at room temperature in a desiccator, giving a yield of ca. 5 g. The metal-free AlPO,-VFI was pre- pared by the same method, but without adding the metal source. The metal impregnated AlPO- M were prepared by stirring AlPO-VFI in a solution of the metal ions (1 mol/L) for 2 h at 40-50C. The AlPO-M were then filtered, washed and dried at room temperature in a desiccator.
2.2. Catalyst characterization
The samples were characterized as synthe- sized by X ray diffraction (XRD) using a Shi- madzu XD-3A diffractometer with Cu K LY radi- ation. Scanning electron micrographs were recorded on a JEOL JSM-T 300 microscope, and the mapping of the metal surface distribu- tion was performed using an energy dispersive X-ray spectrometer (EDS), which provides the semi-quantitative metal content of the samples. Diffuse reflectance UV-visible spectra in the range between 200 and 800 nm were obtained for powdered samples adhering to a sample holder using a Perkin Elmer Lambda-9, 1645 series, spectrophotometer. High proton decou- pled magic angle spinning 27A1 and 3 P NMR spectra were recorded on a Bruker AC 300/P spectrometer. The 27A1 NMR spectra were ob- tained at a frequency of 78.2 MHz and sweep width of 25,000 Hz. Chemical shifts are relative to Al(NO,),. The 31P NMR spectra were ob- tained at a frequency of 121.5 MHz and sweep width of 35,714 Hz. Chemical shifts are relative to 85% H,PO,. Infrared spectra were obtained on a Perkin Elmer 1600 FTIR M-80 Specord spectrophotometer from KBr waffers containing samples of MAPO-VFI. CHN analyses were performed with a Perkin Elmer 2401 analyzer, and the metal contents were determined using a Spectrace TX-5000 X-ray fluorescence spec- trometer, comparing with standard curves pre-
F. J. Luna et al. /Journal of Molecular Catalysis A: Chemical II 7 (1997) 405-411 407
pared from the various metal oxides. Thermo- gravimetric analyses of the MAPO-VFI were carried out with a DuPont 951 instrument.
given as mmol of oxidized products per mmol of metal present in MAPO-VFI.
2.3. Catalytic reactions 3. Results and discussion
Approximately 0.3 g of MAPO-VFI was dried at 80C under vacuum (0.1 mbar) for 2 h. 0.20 g of the dry catalyst was immediately suspended in 15.6 g cyclohexane (99.5%, washed with concentrated sulfuric acid, water, 5% sodium bicarbonate solution, and water and then dis- tilled). 10 mmol tert-butyl hydroperoxide (TBHP) dissolved in 1.1 g cyclohexane, were added and the reaction mixture was magneti- cally stirred in open air for 24 h. Runs with chromium acetylacetonate (Cr(acac>,, Ventron) followed the same procedure. For the autoxida- tion of cyclohexane using CoAPO-VFI, a sus- pension of 0.20 g of the catalyst in 15.6 g of cyclohexane was introduced into a 100 ml auto- clave, pressurized with 25 bar of oxygen, and kept at I 10C for 24 h.
2.4. Chromatographic analysis
The reaction mixture was filtered, approxi- mately 10 mg of cyclooctane (internal standard weighed to 0.1 mg precision) was added, and the sample was diluted with pure cyclohexane (1:5). The samples were analyzed with an HP 5890 series II gas chromatograph equipped with a 4 m X 3.2 mm i.d. column packed with 10% Carbowax 20 M on Chromosorb W-HP, cou- pled to a flame ionization detector, interfaced to an HP Vectra VL pentium workstation. The temperature was programmed at 10C min- from 70 to 170C. The products were identified by co-injection of authentic samples. The effi- ciency with respect to TBHP was calculated taking into account that 1 mol of TBHP is necessary to produce 0.5 mol of cyclohexanone(one), 1 mol of cyclohexene(ene) or 1 mol of cyclohexanol(ol1. The amounts of oxidized products given in the tables have been corrected for blanks. The turnover numbers are
The X-ray diffraction analyses show that the metallaluminophosphates (MAPO) synthesized have the VFI structure and are highly crys- talline. Scanning electron microscopy confirms the presence of a single phase. It also reveals that the MAPO-VFI crystallize in long needles agglomerated into spheres or sphere segments with a radius of 50-75 pm, typical for alu- minophosphates with the VFI structure. The impregnation of AlPO-VFI with the several metal ions does not affect its crystallinity. The UV-visible spectra of Fe- and CoAPO-VFI in- dicate that the metals are tetrahedrally coordi- nated in the framework. On the other hand, the spectrum of VAPO-VFI indicates the presence of VO* cations which are probably coordi- nated to defect sites. The spectrum of TiAPO- VFI shows that, besides the tetrahedrally coor- dinated Ti, some anatase is present in the mate- rial. The UV-visible spectrum of CrAPO-VFI indicates the presence of octahedrally coordi- nated chromium. On the other hand, the FTIR spectrum of this material gives no indication of chromium oxide, suggesting that the chromium substitutes aluminum in the framework and is additionally coordinated to two water molecules, as suggested by Chen and Sheldon . The UV-visible spectrum of MnAPO